and increase its length. Usually, the die is mounted on a draw bench. The starting end of the workpiece is narrowed or pointed to get the end through the die. The end is then placed in grips which pull the rest of the workpiece through the die. Drawing can also be used to cold form a shaped cross-section. Cold drawn cross-sections are more precise and have a better surface finish than hot extruded parts. Inexpensive materials can be used instead of expensive alloys for strength requirements, due to work hardening. Bars or rods that are drawn cannot be coiled; therefore, straight-pull draw benches are used. Chain drives are used to draw workpieces up to . Hydraulic cylinders are used for shorter length workpieces. The reduction in area is usually restricted to between 20% and 50%, because greater reductions would exceed the tensile strength of the material, depending on its ductility. To achieve a certain size or shape, multiple passes through progressively smaller dies and intermediate anneals may be required. Tube drawing is very similar to bar drawing, except the beginning stock is a tube. It is used to decrease the diameter, improve surface finish, and improve dimensional accuracy. A mandrel may or may not be used depending on the specific process used. A floating plug may also be inserted into the inside diameter of the tube to control the wall thickness. Wire drawing has long been used to produce flexible metal wire by drawing the material through a series of dies of decreasing size. These dies are manufactured from a number of materials, the most common being tungsten carbide and diamond. The cold drawing process for steel bars and wire is as follows: Tube lubrication: The surface of the bar or tube is coated with a drawing lubricant such as phosphate or oil to aid cold drawing. Push Pointing: Several inches of the lead ends of the bar or tube are reduced in size by swaging or extruding so that it can pass freely through the drawing die. This is done because the die opening is always smaller in size than the original bar or coil section. Cold drawing, process drawing: In this process, the material is drawn at room temperature. The reduced end of the bar or coil, which is smaller than the die opening, is passed through the die where it enters a gripping device of the drawing